Site-Selective Polyolefin Hydrogenolysis on Atomic Ru for Methanation Suppression and Liquid Fuel Production

Catalytic hydrogenolysis of end-of-life polyolefins can produce value-added liquid fuels and therefore holds great promises in plastic waste reuse and environmental remediation. The major challenge limiting the recycling economic benefit is the severe methanation (usually >20%) induced by terminal C–C cleavage and fragmentation in polyolefin chains. Here, we overcome this challenge by demonstrating that Ru single-atom catalyst can effectively suppress methanation by inhibiting terminal C–C cleavage and preventing chain fragmentation that typically occurs on multi-Ru sites. The Ru single-atom catalyst supported on CeO2 shows an ultralow CH4 yield of 2.2% and a liquid fuel yield of over 94.5% with a production rate of 314.93 gfuels gRu−1 h−1 at 250 °C for 6 h. Such remarkable catalytic activity and selectivity of Ru single-atom catalyst in polyolefin hydrogenolysis offer immense opportunities for plastic upcycling.


Introduction
The ever-growing plastic demands of modern society cause the production of massive solid waste, threatening the environment on which we depend [1][2][3][4]. Polyolefins, used mainly in containers, tubes, and packaging films, account for 57% of the total plastic commodity market [5][6][7]. However, over 85% of waste polyolefins are dumped in landfills or disposed of in environmentally harmful ways (e.g., incineration), contradicting the global sustainability efforts since polyolefin is another form of fossil energy [8][9][10]. The catalytic hydrogenolysis reaction has been developed to convert polyolefins into value-added liquid fuels under mild conditions efficiently [11][12][13][14][15][16]. The H 2 -rich system promotes the hydrogenation of cracked intermediate to form alkanes and suppresses the coke deposition [17]. Up to now, ruthenium (Ru) catalysts manifest the highest catalytic activity for polyolefin hydrogenolysis because they can simultaneously activate all reaction steps, including (a) C−H dehydrogenation, (b) C-C cleavage, and (c) hydrogenation [18][19][20][21][22]. Nevertheless, severe methanation of polyolefins (usually >20%) on multisite Ru has remained a significant challenge to the industrialization of the recycling technology, as it limits the production of higher-value liquid fuels [11,12,23]. While lowering the reaction temperature and increasing H 2 pressure can kinetically alleviate methanation, it is impractical because of the much longer reaction time and higher equipment requirements [24,25].
Recently, geometric control of active metal has been reported to significantly tune the catalytic performance, including activity, selectivity, and stability [26,27]. Smaller metal size and higher disordered properties can boost the production of liquid fuels and suppress the methanation [14,28]. In general, methanation is mainly caused by the dissociation of the terminal C secondary -C primary bond and the fragmentation of the chain on conventional multisite Ru catalysts [25,[29][30][31]. First, the continuous cleavage of terminal carbon from the polymer chain generates methane [14]. Although the limited chain ends in the initial stage do not produce much methane, as the reaction proceeds, a surge in the number of chain ends leads to substantial methane production. Second, simultaneous cracking of 2 adjacent C-C bonds can be catalyzed by clustered Ru atoms. This process is unavoidable on the multisite Ru catalyst surface. Therefore, eliminating the adsorption of polyolefin chains on multisite Ru catalysts or decreasing the energy barrier of internal chain cleavage is expected to suppress the methanation reaction in polyolefin hydrogenolysis.
We show here that the rational design of Ru single-atom catalyst (Ru SAC) provides a solution to the challenge because of its isolated Ru structure and site-selective cleavage mode. Mechanism studies reveal that the internal C-C cleavage is more energy favorable on Ru SAC, thus suppressing the terminal cracking to produce methane; the Ru single-atom cannot provide enough coordination space, thus preventing the continuous breaking of adjacent C-C bonds and inhibiting the production of methane. As a result, the Ru SAC exhibited an ultralow CH 4 yield of 2.2% and the liquid fuel yield of 94.5%. On the basis of this structure-performance relationship, the single-atom system is also universal for efficient upcycling of commercial polyolefins to liquid fuels, offering a promising prospect for plastic upcycling.

Synthesis and morphological characterizations of Ru catalysts
Ru/CeO 2 catalysts with different Ru loadings (0.2, 0.5, 2, and 5 wt%, named as 0.2Ru/CeO 2 , 0.5Ru/CeO 2 , 2Ru/CeO 2 , and 5Ru/CeO 2 , respectively) were synthesized by wet-impregnation method. The RuCl 3 aqueous solution was dropped onto the commercial CeO 2 nanoparticles with an average diameter of ~30 nm, followed by dry, calcination, and reduction steps. Ru contents were determined by inductively coupled plasma optical emission spectrometry with similar values to feed ratios (Table S1). The morphological information of 0.2Ru/CeO 2 was first collected by aberration-corrected high-angle annular darkfield scanning transmission electron microscopy (Fig. 1A). While subtle differences in contrast between Ru and CeO 2 make the observation difficult, no identifiable Ru cluster and nanoparticle indicate its high dispersity, which is consistent with the results of energy-dispersive x-ray spectroscopy (Fig. S1). Interestingly, the other 3 catalysts with much higher Ru ratios share a similar phenomenon: Ru species distribute uniformly on the CeO 2 supports (Fig. S2). The strong metal-support interaction (SMSI) between Ru and CeO 2 should contribute to dispersing Ru atoms [32,33], and such an SMSI effect would also enhance the catalytic stability (see detailed discussion in catalysis part).
The crystal structure of support was also visualized by highresolution transmission electron microscopy (Fig. 1B). The clear lattice fringe with a distance of 0.31 nm is indexed to the (111) facet of CeO 2 . To quantify strain fields in crystalline lattices at a nanoscale resolution, we employed geometric phase analysis (see part 1.3 in the Supplementary Materials). The strain distributions on the single nanoparticle indicate no defect on support after calcination and reduction processes, thus ruling out the substrate effect on the catalytic performance. The high crystallinity of support is also confirmed by the sharp and strong peaks of CeO 2 in the x-ray diffraction (XRD) patterns (PDF no. 34-0394; Fig. S3). The high-resolution XRD pattern of 5Ru/CeO 2 in the range of 36° to 46° (Fig. 1C) also has several weak peaks located at 38.4°, 42.2°, and 44.0°, corresponding to the (100), (002), and (101) facets of hexagonal close packed (hcp) Ru nanocrystals (PDF no. 06-0663). It is worth noting that the signalto-noise ratio of these diffraction peaks decreases sharply with decreased Ru loading, which suggests that the dispersibility of Ru atoms on the CeO 2 surface increases. In particular, the 0.2Ru/ CeO 2 catalyst does not even have an identifiable diffraction signal; thus, it is expected to have a highly dispersed structure.

Electronic structures of Ru catalysts
The electronic property of Ru species plays a significant effect on adsorption/activation/desorption behaviors of each reaction process [34,35]; it could also act as persuasive evidence to identify the single-atom structure [36,37]. Therefore, x-ray photoelectron spectroscopy was performed at Ru 3p orbitals (Fig. S4A), since the Ru 3d orbitals are partially overlapped with C 1s orbital. The fine electronic structure of Ru 3p orbitals shows that the species abundance of Ru 4+ (463.4 eV, oxidative state) and Ru 0 (461.8 eV, metallic state) is related to the loading amount [38]. The proportion of Ru 4+ increases significantly with decreasing loading, while the trend of Ru 0 species is in reverse. The decrease in the loading causes a smaller cluster size, and the aggregated Ru ensembles are broken and isolated, thus promoting the formation of the Ru-O coordination structure. In contrast, the 0.2Ru/CeO 2 catalyst exhibits only an oxidation state (Ru 4+ ) located at 463.4 eV after high-temperature reduction treatment, suggesting its isolated Ru atom structure combined with O from CeO 2 or a subnanometer cluster structure. On the other hand, all Ru/CeO 2 catalysts exhibit almost the same Ce 3d orbitals (Fig. S4B), and the CeO 2 support cannot be reduced before ~350 °C measured by H 2 -temperature program reduction (Fig. S5), which suggests that there are no oxygen vacancies formation during the reduction treatment (300 °C) and hydrogenolysis process (250 °C). The above results exclude the influence of support variation on the catalytic performance.
To further study the precise local electronic structures, we collected x-ray absorption fine structure spectra, including x-ray absorption near-edge structure (XANES) and extended x-ray absorption fine structure (EXAFS), at Ru K-edge. Ru foil and RuO 2 were used as references. As shown in Fig. 1D, with decreasing the Ru loading, the threshold energy (1s → 5p state transition) shifts to the higher energy accompanied by enhanced whiteline intensity, indicating a continuous species evolution from a metallic state to an oxidation state toward RuO 2 . The broadened post-edge feature around 22,160 eV suggests a shrinkage in the cluster size for the samples with lower Ru loading. When the Ru loading is reduced to 0.2 wt%, the blurred spectral feature compared to that of RuO 2 implies its distinct local structure and smaller ensemble size.
Fourier transform (phase uncorrected) is performed on the EXAFS to investigate the local coordination environment of Ru species (Fig. 1E). Remarkably, only the Ru-O scattering path is observed in the 0.2Ru/CeO 2 catalyst, providing solid evidence for the formation of Ru SAC [39,40]. By contrast, the Ru nanocluster catalysts show obvious Ru-Ru scattering paths at ~ 2.4 Å and weak Ru-O scattering paths at ~1.4 Å, confirming their clustered states. Wavelet transform, a parallel mathematical transformation to Fourier transform but with an extra dimension (i.e., energy), is performed upon the EXAFS spectra to precisely identify scattering paths (Fig. 1F) [41]. 0.2Ru/CeO 2 shares the same intensity maximum located at k = 5 Å −1 and R = 1.4 Å with that of RuO 2 , which should be assigned to Ru-O scattering path. However, no features are observed at k = 8.8 Å −1 and R = 2.4 Å, excluding the existence of Ru-Ru scattering path and evidencing its single-atom feature again, whereas other samples with higher Ru loading show similar intensity maxima with that of Ru foil, further demonstrating their cluster intrinsicality. A quantitative analysis was carried out by fitting the EXAFS spectra in the R space (Table S2). In the case of 0.2Ru/CeO 2 catalyst, Ru is only coordinated to O with an average coordination number of 4.59, and no other scattering path can be observed. For all nanocluster catalysts, the Ru coordination numbers are in the range of 6 to 8, which is much lower than that of the fully occupied Ru foil [coordination number (CN) = 12]. Meanwhile, its decreasing trend when reducing Ru content confirms that the Ru cluster size becomes smaller. The Ru-Ru bond distance (2.67 Å) is the same as that of Ru foil. The O coordination numbers are all lower than 2, which should be assigned to the trace amount of oxygen species sitting on the cluster surface.

Hydrogenolysis of polyethylene on Ru catalysts
We first applied n-hexadecane as a model reactant and investigated its hydrogenolysis performance over both Ru SAC and 2Ru/CeO 2 catalyst in a batch stainless steel autoclave (Fig. S6). The 87% of methane yield and nearly 100% of gas yield indicate that 2Ru/CeO 2 tends to cleave the terminal carbons of nhexadecane ( Fig. 2A). Under the same reaction conditions, the Ru SAC provides products with a normal distribution centered on C8, dominated by the internal cracking model. Then, the catalytic hydrogenolysis of low-density polyethylene (LDPE; melting index = 20 to 30 g 10 min -1 ) over various Ru catalysts was systematically tested. The feedstock ratios of Ru to LDPE in all cases were kept at 1:2,000 mg, and the reaction temperature and the H 2 pressure were set to 250 °C and 2 MPa. As shown in Fig. 2B, the Ru SAC exhibits the highest LDPE solid conversion and liquid yield of 97.5% and 94.5%, respectively, as well as the lowest gas yield of 3.05%. Continuous dropped activities and increased overhydrogenolysis tendency are observed with increasing Ru loading. In particular, the solid conversion and liquid product yield of the 5Ru/CeO 2 catalyst drop to only 67.0% and 4.5%, while more than 62.5% of the products are gases. The changing trend of catalytic performance is consistent with the structural evolution from the single-atom structure to clustered Ru aggregates, which confirms that Ru SAC achieves site-selective cleavage of PE chains.
The product distributions of collected gases and liquids on Ru SAC and 2Ru/CeO 2 catalyst with high activities were analyzed by gas chromatography. As seen by visual inspection and statistical analysis of the product distributions (Fig. 2C), the Ru SAC provided a C16-centered distribution of liquid products and the lowest methane yield of 2.2%, whereas a broad C18-centered liquid distribution and 21.1% of methane were received from 2Ru/CeO 2 . The relatively narrow product distribution and lower methane yield obtained from Ru SAC indicate the internal C-C cleavage model on the Ru single-atom site, leading to the rapid shrink of chain distribution.
We further compare the catalytic performance of our Ru catalysts with that of the reported ones. The production rate of liquid fuels (in grams of fuels per gram of Ru per hour) is defined to evaluate various Ru catalysts ( Fig. 2D and Table S3). Specifically, the Ru SAC has the lowest gas yield of 3.05% and the highest liquid fuel production rate of 314.93 g fuels g Ru −1 h −1 , which is far superior to other reported Ru catalysts. The 2Ru/ CeO 2 catalyst has a similar gas yield of 23.1% to the reference nanocluster catalysts, confirming that our results are reasonable. Further increasing the Ru loading (5Ru/CeO 2 ) leads to a dropping in solid conversion and more tendency to methanation (gas yield of 62.5%). It is mainly due to less exposed active sites and the formation of more Ru-Ru sites to crack the terminal C-C bonds. Therefore, benefiting from the maximum atom utilization and selective cracking model, the activity and selectivity of Ru SAC are significantly improved compared to those of nanocluster catalysts.

Hydrogenolysis mechanism of PE on Ru SAC
The in-depth mechanism investigation of the reaction pathways on Ru SAC and 2Ru/CeO 2 is further explored by time-dependent experiments. In the initial hydrogenolysis process (less than 2 h), Ru SAC converts waste PE to products with flat and broad carbon distribution (Fig. 3A), indicating the random cleavage of the internal C-C bonds on the Ru single-atom structure. In contrast, the 2Ru/CeO 2 nanocluster catalyst exhibits an uneven carbon distribution with both high contents of alkanes of C28 to C35 and CH 4 (5.5%; Fig. 3B). Importantly, in the next 2 h, with a dramatic increase in solid conversion, the product distribution on the Ru SAC is shifted to the lower carbon chain with a carbon distribution center at C14, whereas the 2Ru/CeO 2 catalyst still continuously produces C28 to C35 and CH 4 . Further extending the reaction time makes the product distribution on Ru SAC concentrate more on C14, while those C28 to C35 are digested to generate CH 4 on 2Ru/CeO 2 surface dramatically. The above results again confirm that the Ru SAC prefers to cleave internal C-C bonds and the terminal cleavage model on multisite Ru catalysts is dominated.
In addition, we perform the hydrogenolysis behavior on different light alkanes to further probe the mechanism. When all reaction conditions are kept the same, the CH 4 yields in different cleavage models are sensitive to the number of terminal sites (determined by molecular weight) in the reaction system. As displayed in Fig. 3C, the CH 4 yield on the 2Ru/CeO 2 catalysts shows a more obvious sensitivity to the carbon-chain length that the CH 4 yield dramatically increases from 8.9% in n-decane hydrogenolysis to 12.4% in n-hexadecane hydrogenolysis, which verifies its terminal cracking model again. Remarkably, the Ru SAC maintains stable CH 4 yields of 0.4% to 1% during the hydrogenolysis of alkanes with different carbon numbers, confirming its inertness to terminal C-C dissociation.
To deeply explore the relationship between Ru structure and CH 4 selectivity in the hydrogenolysis process, we performed density functional theory (DFT) calculations to understand the cleavage models of terminal/inner carbons from the polymer chain. Here, we have constructed single-atom (one Ru atom is boned with 3 surface O atoms and one O atom) and multi-Ru (Ru trimer; each Ru atom is bonded with one surface O atom) sites anchored on the CeO 2 (111) surface to simulate the Ru SAC and Ru nanocluster catalyst. The n-hexane is employed to simulate the long-chain alkane for simplicity. Considering the C-H bond in n-hexane is easy to break on Ru atom with the calculated barriers of 0.45 eV for the terminal C1 and 0.54 eV for the inner C3 (Fig. S7), respectively. Thus, hexene is chosen as the reactants to study the cleavage mode on Ru SAC and Ru 3 /CeO 2 .
For the Ru single-atom model, when one carbon atom in hexene is bonded with a single Ru atom, Ru SAC prefers to cleave the inner C3-C4 bond with the barrier of 1.20 eV, remarkably lower than the barrier of 1.72 eV to break the terminal C1-C2 bond in hexane (Fig. S8A). A similar result is founded when Ru atom is bonded with 2 contiguous carbon atoms (Fig. S8B). Therefore, on Ru SAC, the n-hexane tends to dehydrogenate into 3-hexyl intermediate and cleaves the inner C-C bond in hexane, which efficiently suppresses the CH 4 formation and facilitates the liquid fuel production. Conversely, as shown in Fig. S9A, Ru 3 /CeO 2 prefers to cleave the terminal C1-C2 bond with the barrier of 1.54 eV rather than the inner C3-C4 bond of 1.75 eV. The *CH 2 intermediate is formed after the C1-C2 bond breakage, implying the possible production of CH 4 . The similar results are also obtained in the cleavage of hexyne as alkyne intermediates (Fig. S9B), indicating a favorable terminal C-C cleavage mode on multi-Ru site. Combined with our experimental results, in the initial stage of alkane/polyolefin hydrogenolysis, the terminal cracking is limited by the minimal sites, and the hydrogenolysis process may undergo the random inner cracking. However, as the reaction proceeds, rapidly enhanced terminal C secondary -C primary sites would cause serious energy-favorable methanation. The theoretical results have demonstrated that the catalytic mechanism of n-hexane on single-atom Ru 1 /CeO 2 and Ru 3 /CeO 2 surfaces is different and the single metal Ru site could inhibit the fragmentation reaction, promoting the liquid fuel production (Fig. 3D).
In addition, the whole reaction paths of n-hexane dissociated on the Ru SAC surface are shown in Fig. S10, and n-hexane first adsorbs on the Ru SAC, where the C3 atom locates on the top of the Ru atom. Under the activation of single-atom Ru, the inner C-H bond in n-hexane is first cleaved by overcoming a low barrier of 0.54 eV (S0 to S1), and then breaking the C3-C4 bond needs to overcome a barrier of 1.41 eV (S1 to S2) with the formation of *CH 3 CH 2 CH 2 and *CHCH 2 CH 3 intermediates. After that, the hydrogenation of *CH 2 CH 2 CH 3 generates desorbed propane (S2 to S3) with a low barrier of only 0.48 eV, suggesting that the subsequent hydrogenation and desorption processes are facile once the C-C bond is activated. Our theoretical results further confirm that the internal C-C bond cleavage in n-hexane on Ru SAC is energetically preferred, which could successfully suppress the CH 4 production and boost the production of liquid fuels with high selectivity.

Controlling carbon distribution of products
The pursuit of high recycling benefits from waste plastics and controlling product distribution are conducive to technology industrialization. Time-dependent experiments on LDPE hydrogenolysis were evaluated over Ru SAC and 2Ru/CeO 2 . After 2 h of reaction, 55% of PE has been converted to liquid alkanes (Fig. 4A). These liquid products are good solvents for PE and reduce the system viscosity, thereby enhancing mass transfer efficiency and leading to a dramatic increase in subsequent catalytic activity (during 2 to 3 h) [42,43]. The residual solids are further converted to lower alkanes in the subsequent reaction with nearly 100% of solid conversion after 6 h. Although further prolonging the reaction time increases the gas yield slightly but it remains below 10%, the large change in the carbon distribution of liquid fuel allows precise product control and value optimization. In our case, the liquid fuels ranging from C5 to C35 are divided into C5 to C12 (gasoline), C13 to C22 (diesel), and C23 to C35 (liquid wax). In general, gasoline possesses a higher value than diesel and liquid wax; thus, the hydrogenolysis process should be deepened while maintaining a low gaseous yield. As the reaction progresses to 24 h, the half-peak width of the fitted distributions becomes more concentrated, and finally, the carbon-chain center gradually shifts to C11 (Fig.  4B and Fig. S11), receiving 63% of gasoline yield (Fig. S12). Notably, while prolonging the reaction time of the 2Ru/CeO 2 catalyst can also modulate the carbon distribution of liquid products, it leads to severe methanation, which is not conducive to the economic benefits (Fig. S13).
Corresponding economic analysis (see details in part 1.4 in the Supplementary Materials) of the products is evaluated to figure out the recycling benefits during the hydrogenolysis process. As shown in Fig. 4C, with above 90% of solid conversion of LDPE (reaction time > 4 h), the value of the overall products shows a sharp increase from 4 to 8 h, mainly due to the substantial conversion of liquid wax to the higher-value diesel and gasoline. After 8 h of reaction, the conversion of diesel to gasoline dominates the reaction. Although the values of the 2 oils are relatively close, the economic benefits only display a slow increase when prolonging the reaction time to 20 h. Noted that the subsequent overhydrogenolysis of gasoline would lead to the formation of undesired gaseous products (Fig. 4A), resulting in a decrease in product value.
While reasonable optimizations of reaction parameters are usually used to maximize the economic benefit of a specific reaction, it also affects the total energy consumption. Here, the industrial hydrogenolysis process of PE is simulated by treating 60,000 tons of PE per year ( Fig. S14; see detailed flow diagram and parameters in Fig. S15 and Table S4). In a typical process, the waste PE, catalyst, and H 2 are pumped into the reactor with 100% of solid conversion to produce the C1 to C35 hydrocarbons, followed by the separation of gases including H 2 and C1 to C12 and the nongaseous mixture of catalyst and C13 to C35 hydrocarbons. Subsequently, the gas components pass through 2 consecutive separators to receive the H 2 , natural gas (C1 to C4), and gasoline (C5 to C12). A solid-liquid filter is used in another products line to separate the solid catalyst and the liquid C13 to C35 hydrocarbons. In addition, the liquids are transported to a rectifying tower to vaporize the diesel product (C13 to C22) with a purity of 99% and retain the liquid wax (97%). The energy consumption of each equipment and total process are calculated on the basis of the PE hydrogenolysis performance of Ru SAC for 6 h. Compared to the 3 separators and the rectifying tower, the reactor consumes the most energy which is 9.25 × 10 3 GJ, accounting for 90.25% of the whole process ( Fig. S14 and Table S5). The calculations also show that the energy consumptions for converting PE into different products (C5 to C12, C13 to C22, or C23 to C35) are dramatically different (Table S6). Although more gasoline can be obtained by prolonging the reaction time, it also leads to more energy consumption without substantially increasing the product's value (Fig. S12). Therefore, simply prolonging the reaction time to increase gasoline yield is not conducive to increasing profits but will consume a lot of energy. The development of efficient selective catalysts can fundamentally yield the target product.
Catalyst stability and recoverability are also important criteria for industrial polyolefin hydrogenolysis. The catalytic stability of the Ru SAC was also tested. In detail, the spent Ru SAC (named Ru SAC-S) were centrifugally collected and thoroughly washed 5 times with hot toluene. The Ru SAC-S with ~10% of weight loss was then mixed with fresh quantitative catalysts for the next round of hydrogenolysis test. Over 5 hydrogenolysis cycles, Ru SAC-S exhibits almost constant catalytic performance with ~97% of solid conversion of LDPE, ~94% of liquid yield, and ~3% of gaseous yield, indicating its excellent stability (Fig. 5A). The chemical structures of the Ru SAC-S after 5 cycles were further characterized by XANES and EXAFS (Fig. S16). The spent catalyst shows only Ru-O coordination feature and a similar whiteline intensity with these of the fresh Ru SAC, indicating the stable single-atom structures. The SMSI between Ru and CeO 2 can effectively suppress the metal sintering and leaching during the high-temperature reaction, resulting in an ultrastable hydrogenolysis performance of Ru SAC.

Upcycling of commercial polyolefins
The feasibility and universality of Ru SAC on catalytic hydrogenolysis are investigated by degradation of high-density polyethylene (HDPE), polypropylene (PP), and commercial polyolefin waste ( Fig. 5B and C). In terms of topological structure, the HDPE has a linear chain structure, while more short branches are derived in the LDPE. Under the same reaction condition, the solid conversion of HDPE reaches 100%, and the gas yield is 7.5%, exhibiting a slight overhydrogenolysis phenomenon, which indicates that catalytic hydrogenolysis of HDPE has a higher activity than that of LDPE. The low activity of LDPE may be caused by the steric hindrance of branches, which does not favor the chain adsorption on catalysts [19,30]. In addition, the methyl side groups make the breakage of backbone C-C bonds more difficult [19,44], thus requiring a longer catalytic reaction time (18 h) to achieve high solid conversion. Interestingly, the gas yield is almost zero compared to the common ~30% [12,45]. According to previous works, the PP contains many pendant methyl groups [46,47], and the removal of these groups would yield more methane than that in PE hydrogenolysis. Combined with the unique cleavage mechanism of Ru SAC proposed in the PE hydrogenolysis, we speculate that the hydrogenolysis of PP may also follow the internal C-C breakage model (right panel in Fig. S17).
Notably, since the polyolefin wastes are more complex than raw materials and always contain various additives and impurities, the hydrogenolysis of commercial plastics, including LDPE bags and HDPE and PP bottles, on Ru SAC was also demonstrated. The commercial materials were cut into squares shapes with dimensions of 5 × 5 mm for subsequent use. Overall, the Ru SAC shows high solid conversions and liquid yields over 80% and gas yields below 10% in the degradation of various commercial polyolefin wastes. Combined with the high selectivity, good stability/recyclability, and high atomic usage, the polyolefin hydrogenolysis system assisted by Ru SACs holds a great promise for promoting sustainable plastic upcycling.

Discussion
Summarily, we have synthesized and confirmed that Ru SAC can selectively cleave internal C-C bonds in PE hydrogenolysis, whereas the terminal C-C cracking and fragmentation tend to occur at multi-Ru sites. As a result, the Ru SAC shows a production rate of 314.93 g fuels g Ru −1 h −1 with an ultralow gaseous yield of 3.05% and a liquid fuel yield of 94.5%, which all are much better than those of other reported Ru catalysts. We have further demonstrated that the single-atom system is also universal and efficient for upcycling commercial polyolefin commodities, giving an enormous potential for industrialization. This work also offers an in-depth understanding of the structure-performance relationship between active sites and polyolefin hydrogenolysis. Our investigation of the structure-performance relationship only distinguishes the catalytic mechanism of SAC and multisite Ru catalyst, while a crucial goal for sustainable polyolefin upcycling is to develop an efficient catalyst, which corresponds to our discussion on reaction engineering parameters. In general, the catalytic performance of SAC can be modulated by tuning its electronic structure, coordination environment, and interaction with support. Therefore, rational design and study of SAC with further improved performance toward polyolefin upcycling are worth more attention.

Synthesis of Ru/CeO 2 catalysts
All Ru/CeO 2 catalysts were prepared by a well-established wetimpregnation method. The mass fractions of Ru were kept at 0.2, 0.5, 2, and 5 wt%. In a typical synthetic process, certain amounts of RuCl 3 aqueous solutions were dropped onto the CeO 2 powder in a 20-ml bottle, which was put on a hotplate at 80 °C under magnetic stirring of 400 rpm until the slurry formation, followed by the dry and age in an oven at 80 °C for 12 h. Afterward, the obtained samples expected 0.2Ru/CeO 2 were calcinated in a muffle furnace at 500 °C for 2 h. Prior to catalytic hydrogenolysis, all samples were reduced in a 5%H 2 /Ar (100 ml min −1 ) gas flow at 300 °C for 2 h.

Catalytic evaluation and product determination
The hydrogenolysis experiments were performed in a 100-ml batch stainless steel autoclave with magnetic stirring equipment. The polymers/alkanes and catalysts were physically mixed and put into the reactor. Before catalytic tests, the reactor was preflushed with H 2 under 2 MPa for 5 cycles, followed by the H 2 pressurization at a total pressure of 2 MPa, and then sealed the reactor. The stirring rate during the reaction was kept at 400 rpm. After the reaction and temperature cooling down to room temperature, the gaseous products were collected by a gas sampling bag. The liquid products and solid residuals were respectively dissolved and dispersed in 30 ml of toluene and stored in the refrigerator, making the liquid of high molecular weight (carbon number > 35) is precipitated. Afterward, the solid residue and liquid product are then separated by a refrigerated centrifuge. The solid residuals were washed with n-hexane for 3 times and further dried in the oven at 80 °C for 12 h. For the product distribution, the gaseous (C1 to C4) and liquid (C5 to C35) products were quantitatively analyzed by 2 gas chromatographs with flame ionization detector using TM-Al 2 O 3 /S and HP-1 capillary columns, respectively. The catalytic performance was gravimetrically calculated by the following equations, the product yields are calculated on a carbon basis:

Reusability test
The solid residuals were dispersed in a hot toluene solution in a 20-ml bottle on a hotplate to dissolve the hydrocarbons. The spent catalyst was separated by centrifugation. Repeat the process 5 times to obtain the clean spent catalyst. In general, the loss of the catalyst each time was ~10%. For the new hydrogenolysis test, the catalyst was composed of all spent catalyst and partial fresh catalyst.

Data Availability
All data needed to evaluate the conclusions in the paper are present in the paper and/or the Supplementary Materials. Additional data related to this paper may be requested from the authors.

Supplementary Materials
Experimental Procedures.  Fig. S10. Catalytic reaction path and barriers of n-hexane dissociation on Ru SAC from DFT calculations. Fig. S11. Distribution of nonsolid products on LDPE hydrogenolysis over Ru SAC from 2 to 24 h. Fig. S12. Time-dependent analysis. Product yields of gasoline (C5 to C12), diesel (C13 to C22), and liquid wax (C23 to C35) over Ru SAC on LDPE hydrogenolysis for 4 to 24 h. Fig. S13. Time-dependent analysis of Ru non-SAC for 2 to 6 h. Fig. S14. Schematic illustration of the industrial process of PE hydrogenolysis by Aspen Plus software. Fig. S15. Detailed flow diagram of industrial PE hydrogenolysis based on the simulation through Aspen Plus software. Fig. S16. Electronic structure of Ru SAC-S. Fig. S17. Plausible mechanism of C-C hydrogenolysis of PP over Ru nanoparticle and Ru SAC. Table S1. The elemental compositions of Ru/CeO 2 catalysts measured by inductively coupled plasma optical emission spectrometry. Table S2. Fitting results of EXAFS spectra.